Different Shaped Nanoparticles
Importance of Core/Shell Nanoparticles
Classes of Core/Shell Nanoparticles
Inorganic/Inorganic Core/Shell Nanoparticles
Inorganic/Organic Core/Shell Nanoparticles
Organic/Inorganic Core/Shell Nanoparticles
Organic/Organic Core/Shell Nanoparticles
Approaches for Core/Shell Nanoparticle Synthesis
Techniques, classification, and mechanism of core/shell nanoparticle synthesis
Nanomaterials have, by definition, one or more dimension in the nanometer scale
(100 nm) range and subsequently show novel properties from their bulk materials.
The most important characteristics, among many others, on a nanoscale are as
First, the small size of the particles, which leads to an increased surface area to
volume ratio and as a result the domain where quantum effects predominate is
Second, the increasing surface area to volume ratio leads to an increase in the
dominance of the surface atoms of the nanoparticle over those in its interior.
However, broadly these all techniques essentially fall into three categories: (i)
condensation from vapor, (ii) synthesis by chemical reaction, and (iii) solid-state
processes such as milling.
By using the above-mentioned techniques, not only pure nanoparticles but also
hybrid or coated nanoparticles (with hydrophilic or hydrophobic materials depending
on the suitability of the applications) can be synthesized.
Figure: Different core/shell nanoparticles:
(a) spherical core/shell nanoparticles;
(b) hexagonal core/shell nanoparticles;
(c) multiple small core materials coated by
single shell material;
(d) nanomatryushka material;
The properties of nanoparticles are not only
size dependent but are also linked with the
For example, certain properties of magnetic
nanocrystals such as the blocking
temperature, magnetic saturation, and
permanent magnetization are all dependent
on particle size, but the coercivity of the
nanocrystals totally depends on the particle
chemical properties such as catalytic
activity and selectivity, electrical and
optical properties, sensitivity to surfaceenhanced Raman scattering (SERS)
and the plasmon resonance and melting
point are also all highly shape-
IMPORTANCE OF CORE/SHELL
Emerged at the frontier between materials chemistry and many other fields,
such as electronics, biomedical, pharmaceutical, optics, and catalysis.
Core/shell nanoparticles are highly functional materials with modified
Because of the shell material coating, the properties of the core particle such
as reactivity decrease or thermal stability can be modified, so that the overall
particle stability and dispersibility of the core particle increases.
The purpose of the coating on the core particle are many fold, such as surface
modification, the ability to increase the functionality, stability, and dispersibility,
controlled release of the core, reduction in consumption of precious materials,
and so on.
Nano- and microsized hollow particles are used for different purposes such as
microvessels, catalytic supports, adsorbents, lightweight structural materials and
thermal and electric insulators.
CLASSES OF CORE/SHELL
NANOPARTICLES be broadly defined as
The core/shell type nanoparticles can
comprising a core (inner material) and a shell (outer layer material).
These can consist of a wide range of different combinations in
close interaction, including
The choice of shell material of the core/shell nanoparticle is generally
strongly dependent on the end application and use.
Multiple core core/shell particles are formed when a single shell
material is coated onto many small core particles together
CORE/SHELL the silica coating compared with other inorganic
The most basic advantages of
(metal or metal oxide) or organic coatings are as follows:
It reduces the bulk conductivity and increases the suspension stability of the core
In addition, silica is the most chemically inert material available; it can block the
core surface without interfering in the redox reaction at the core surface.
Silica coatings can also be used to modulate the position and intensity of the
surface plasmon absorbance band since silica is optically transparent.
As a result, chemical reactions at the core surface can be studied spectroscopically.
Gold coating on any particles enhances many physical properties, such as the
chemical stability by protecting the core material from oxidation and corrosion, the
biocompatibility, the bioaffinity through functionalization of amine/thiol terminal groups,
and the optical properties.
Other shell metals such as Ni,Co,Pd,Pt and Cu are also important for some specific
applications in the field of catalysis, solar energy absorption, permanent magnetic
Similar to the size-dependent color of
pure gold nanoparticles, the optical
response of gold nanoshells depends
dramatically on the relative size of the
core nanoparticle as well as the
thickness of the gold shell.
By varying the relative core and shell
thicknesses, the color of such gold
nanoshells can be varied across a broad
range of the optical spectrum spanning
the visible and the near-infrared spectral
regions as shown in Figure.
Nanoparticles- particles are used for
enhancement of optical properties, lightemitting devices, nonlinear optics,
efficiency of either solar cells or the
storage capacity of electronics devices,
In Type I, this category, the energy band gap of
the shell material is wider than the band gap of
the core material.
The electrons and holes are confined within the
core area because both the conduction and the
valence band edges of the core are located
within the energy gap of the shell.
As a result, the emission energy, hωPL, is
determined by the energy gap of the core
The shell is used to passivate the surface of
the core with the goal of improving its overall
Another role of the shell is to separate the more
optically active core surface from its surrounding
The wider band gap shell material increases
the stability against photobleaching of the
However, the increasing thickness of the shell Figure:
layer reduces the material surface activity of the semiconductor/semiconductor
core surface; as a result, quantum yield also core/shell materials. Sem1 = core material, Sem2 = shell
These types of semiconductor particles
especially those made from CdSe/CdS,
In type II, the narrower band gap shell
material is grown over the wider band gap
In this case, both hole and electron
charges are partially localized on the shell
materials and emission wavelengths can be
tuned by changing the thickness of the shell.
Within this category, the most extensively
studied systems are CdS/CdSe and
Here the types of particles have low
quantum yields and higher resistance
against photobleaching, whereas the
quantum yield can be improved by coating
another semiconductor material of a wider
For example, the quantum yield (QY) of
CdSe- coated CdS core/shell nanoparticles
in aqueous media is 20%.
Figure: (a) Schematic diagram of an onion-like structure
of alternate multifold CdS (1.7 eV)/CdSe (2.5 eV)
structure and its corresponding energy diagram.
(b) UV-vis absorption and PL spectra.
(c) Corresponding luminescence image for the samples
under UV lamp irradiation.
Inorganic/organic core/shell nanoparticles are made of metal, a metallic compound,
metal oxide, or a silica core with a polymer shell or a shell of any other high density
The advantages of the organic coating on the inorganic material are many fold.
One example is the fact that the oxidation stability of the metal core is increased
when otherwise the surface atoms of the metal core can be oxidized to the metal oxide
in a normal environment.
In addition, they exhibit enhanced biocompatibility for bioapplications.
The polymer-coated inorganic materials have a broad spectrum of applications,
ranging from catalysis to additives, pigments, paints, cosmetics, and inks.
In many applications, the particles are coated to stabilize them in the suspension
media, and the stability of such a colloidal suspension depends mainly on the
attractive and repulsive forces between the particles.
There are four different types of forces: (i) van der Waals forces, (ii) induced short-
Magnetic nanoparticles with any polymer coating are used mainly for magnetic
recording, magnetic sealing, electromagnetic shielding, MRI, and especially in the
biological field for specific drug targeting, magnetic cell separation, etc.
Dextran, a polysaccharide polymer composed of exclusively R-D-glucopyranosyl
units with varying degrees of chain length and branching, is also widely used as a shell
Dextran is used as a polymeric shell because of its high biocompatibility.
It in turn increases the biocompatibility of the magnetic nanoparticles to the extent
that they can be used in in vivo applications.
Side-chain-functionalized dextran coated ultrasmall superparamagnetic iron oxides
(USPIO) show a prolonged blood residence time, which allows these USPIO particles
to access the macrophages located in deep pathological tissues (such as lymph
nodes, kidney, brain, osteoarticular tissues, etc.).
Dextran-coated Fe nanoparticles are also used for labeling red blood cells (RBC) in
cell separation studies using high gradient magnetic chromatography (HGMC).
The most common polymers used as organic coatings on silica cores are
poly(3aminophenylboronic acid),348 and poly(vinyl chloride) (PVC) conductive polymers
such as polyaniline (PANI), polypyrole (PPy), and polythiophene (PTh), .
Natural polymers such as cellulose
Polymer-coated AgCl nanoparticles are useful for sensor applications.
Polymer-coated CaCO3 shows improved mechanical properties as a filler
material and is useful in different applications.
Polystyrene-coated CaCO3 is widely used in the manufacture of paint, paper,
rubber, plastics, etc.
It was found that instead of pure CaCO3, a poly(butylene tetraphthalate) (PBT)
coating on stearic acid-modified CaCO3 improves the mechanical, thermal, and
structural properties of the CaCO3.
As an example, the tensile strength of stearic acid-modified CaCO3 increases
from 56 to 58.9 MPa because of the PBT coating; 80% weight fraction of the
CORE/SHELL NANOPARTICLES such as
The core of this particular class of core/shell nanoparticles is made of a polymer,
polystyrene, poly(ethylene oxide), polyurethane, poly(vinyl benzyl chloride), poly(vinyl
acrylonitrilebutadienestyrene, poly- (styreneacrylic acid), and styrenemethyl methacrylate.
The shell can also be made from different materials, such as metals, metal oxides, metal
chalcogenides or silica.
The inorganic material, especially a metal oxide coating on an organic material, is beneficial
in several respects, such as increased strength of the overall material, resistance to
oxidation, thermal and colloidal stability, and abrasion resistance.
At the same time, these particles also show polymeric properties such as excellent optical
properties, flexibility, and toughness, and in addition they can improve the brittleness of the
Phadtare et al. synthesized gold-coated polyurethane microsized core/shell particles for
applications where biocatalytic activity was required in such applications as pepsin digestion.
Another interesting application of these types of particles is for the synthesis of hollow
inorganic particles by using an organic material as the sacrificial core.
In this category, both the core and shell particles are made of a polymer or another
These classes of particles are known as “smart particles” and have a wide range of
applications in different fields, such as drug delivery, biosensing, chemical separation,
biomaterials, and catalysis.
The advantages of having a polymer coating on another polymer is to modify the
physical properties of the overall material, such as toughness or the glass transition
The glass transition temperature is an important characteristic of a polymer because
below this temperature polymers are in what is called a “glassy state”.
When the temperature of the material crosses the glass transition temperature, the
mechanical properties of the polymers change from those of a glass (brittle) to a
rubber (elastic) material.
For example, a polymer coating on a polymer with a different Tg is used to modify
latex-based paints. A high Tg core material has the impact of improving the mechanical
Polymer/polymer core/shell particles are also extensively used for controlled
drug release applications in in vivo systems because of their good
biodegradable and drug encapsulation property.
Poly(D,L-lactic-co-glycolide) (PLGA) is a biodegradable organic polymer with
a high capacity for encapsulating hydrophobic drugs.
C-dots coated with a polymer are promising as tools for sensing and imaging
subcellular agents because they can be delivered into the cell cytoplasm.
APPROACHES FOR CORE/SHELL
NANOPARTICLE SYNTHESISinto two categories: “topApproches for nanomaterial synthesis can be broadly divided
down” and “bottom-up”.
The “topdown” approach often uses traditional workshop or microfabrication methods
where externally controlled tools are used to cut, mill, and shape materials into the desired
shape and order.
For example, the most common techniques are lithographic techniques (e.g., UV, electron
or ion beam, scanning probe, optical near field), laser-beam processing, and mechanical
techniques (e.g., machining, grinding, and polishing).
“Bottom-up” approaches, on the other hand, exploit the chemical properties of the
molecules to cause them to self-assemble into some useful conformation.
The most common bottom-up approaches are chemical synthesis, chemical vapor
deposition, laser-induced assembly (i.e., laser tapping), self-assembly, colloidal aggregation,
film deposition and growth etc.
However, the bottom-up approach can produce much smaller sized particles and has the
potential to be more cost-effective in the future because of the advantages of absolute
precision, complete control over the process, and minimum energy loss compared with that of
a topdown approach.
TECHNIQUES, CLASSIFICATION, AND
MECHANISM OF CORE/SHELL
NANOPARTICLEare synthesized using a two-step process, first synthesis of core
In general, core/shell nanoparticles
and second the synthesis of the shell.
The synthesis techniques of core/shell nanoparticles can be classified into two types depending on
the availability of core particles:
(i) the core particles are synthesized and separately incorporated into the system with proper
surface modification for coating the shell material;
(ii) the core particles are synthesized in situ, and this is followed by coating of the shell material.
The basic advantage of external core synthesis is the fact that core particles are available in pure
form and hence there is less possibility of impurities on the core surface.
Whereas, in in situ synthesis, the main problem is that some impurity from the reaction media may
be trapped between the core and shell layer.
The most important step during synthesis of core/shell particles is to maintain uniform coating and to
control the shell thickness.
Some of the various synthetic methods for core/ shell particles used by different research groups are
precipitation, polymerization, microemulsion, sol-gel condensation, layer by layer adsorption
Figure: Schematic diagram for Cu/Cu2O core/shell nanoparticle synthesis using the thermal
decomposition of a metal organic complex
The main difficulties are
(i) agglomeration of core particles in the reaction media,
(ii) preferential formation of separate particles of shell
material rather than coating the core,
(iii) incomplete coverage of the core surface, and
(iv) control of the reaction rate.
Fig. Silica/PT core/shell nanospheres: (a) a schemetic
illustration of silica/PT core/shell nanoparticles fabrication using
seeded polymerization , and (b–d) SEM images with different
diameters of silica nanoparticles (insets: TEM images of a single
core/shell nanoparticle , scale bar indicates 10 nm): (b) 11 nm, (c)
16 nm, (d) 26 nm.
Step 1. Mixing. For the first method, the suspension of colloidal powder or sol is formed by
the mechanical mixing of colloidal particles in water at a suitable pH without any
precipitation. For the other two methods, metal alkoxide or metal salt are used as a
precursors, which are hydrolyzed to form hydrated metal hydroxides in the presence of water,
which subsequently undergo condensation to form an oxo bridge (MOM). When sufficient
MOM bonds are formed in a region, then they cooperatively respond to form colloidal
particles or sol. The size of the particles depends on the pH of the medium and the ratio of
water to metal alkoxide or metal salt.
Step 2. Casting. Since the sol is a low-viscosity liquid, it can be cast into a mold.
Step 3. Gelation. With time, the colloidal particles and condensed species link together to
Step 4. Aging. The aging of the gel involves maintaining the cast object for a period of time,
completely immersed in liquid for polycondensation, syneresis, coarsening and phase
Step 5. Drying. The liquid is removed from the interconnected pore network during the
Step 6. Dehydration or chemical stabilization. The surface metal-hydroxide bonds are
removed in this step, and the material is converted into a stable ultraporous solid with
sufficient interconnected porosity, optical transparency, and good mechanical strength.
Step 7. Densification. After dehydration, solid materials are heated at high temperatures to
increase density by reducing the internal porosity.
During the last four steps, the shrinkage and densification occurs because of
(1) capillary contraction, (2) condensation, (3) structural relaxation, and (4) viscous sintering.
In the first step, the rate of hydrolysis of metal or metalloid alkoxide or salt is affected by
some physical parameters such as (i) pH, (ii) substituents, (iii) solvent, and (iv) water.
Figure: Reaction steps for
nanoparticle formation by
synthesis of CdS/S core/shell
By modulating the size, shape, and
material of the core, the optics can
be tuned and optimized for use in
optical devices and applications
such as LEDs, detectors, lasers,
phosphors, and photovoltaics.
Biomedical Applications- Controlled Drug Delivery and
Replacement, Support, and Tissues
The future generations of core/shell nanoparticles will exhibit many new properties that will
surely result in new applications with improved performance.
Generally core/shell nanoparticles are well-known for better stability, for being able to
protect the core material from the surrounding environment, for improved physical and
chemical properties, for improved semiconductor properties, for easy biofunctionalization, etc.
Most of the recent exciting discoveries show that there is tremendous scope in biomedical
applications such as controlled drug delivery and release, targeted drug delivery, bioimaging,
cell leveling, biosensors, diagnostics, immunoassays, and many more.
In the near future, the development of new materials has the potential for improving the
treatment of cancer and many other life threatening diseases.